Presentation on theme: "1 Dr.Apiwat Muttamara. Outline Equipment and process steps Design for Part Design for manufacturing, tooling and defects."— Presentation transcript:
1 Dr.Apiwat Muttamara
Outline Equipment and process steps Design for Part Design for manufacturing, tooling and defects
THERMOPLASTIC, THERMOSET: Thermoplastics are resins that can be reground after molding, and molded again. Thermoplastic are often compared to Wax. Thermosets can be molded once only; they tend to be denser materials for special purposes, thermosets are often compared to an egg; once the egg is hard boiled it can't be returned to a liquid and recooked as sunny side up.
Plastics Processing: Injection Molding
Mold Structure: Parting line A dividing line between a cavity plate and a core plate of a mold. - Make a parting line on a flat or simple-curved surface so that flash cannot be generated. - Venting gas or air.
Two plate mold One parting line
Three plate mold Two parting lines
Gate -Delivers the flow of molten plastics. -Quickly cools and solidifies to avoid backflow after molten plastics has filled up in the cavity. -Easy cutting from a runner -Location is important to balance flow and orientation and to avoid defects. L = 0.5-0.75 mm h(thickness) = n.t W= n A 1/2 30
Runner cross section Runner cross section that minimizes liquid resistance and temperature reduction when molten plastics flows into the cavity. - Too big - Longer cooling time, more material, cost - Too small - short shot, sink mark, bad quality - Too long - pressure drop, waste, cooling Hot runner, runnerless mold
Runner balancing Balanced Not balanced
Defects Molding defects are caused by related and complicated reasons as follows: * Malfunctions of molding machine * Inappropriate molding conditions * Flaws in product and mold design * Improper Selection of molding material
Weldline This is a phenomenon where a thin line is created when different flows of molten plastics in a mold cavity meet and remain undissolved. It is a boundary between flows caused by incomplete dissolution of molten plastics. It often develops around the far edge of the gate. Cause Low temperature of the mold causes incomplete dissolution of the molten plastics. Solution Increase injection speed and raise the mold temperature. Lower the molten plastics temperature and increase the injection pressure. Change the gate position and the flow of molten plastics. Change the gate position to prevent development of weldline.
Flashes Flashes develop at the mold parting line or ejector pin installation point. It is a phenomenon where molten polymer smears out and sticks to the gap. Cause Poor quality of the mold. The molten polymer has too low viscosity. Injection pressure is too high, or clamping force is too weak. Solution Avoiding excessive difference in thickness is most effective. Slow down the injection speed. Apply well-balanced pressure to the mold to get consistent clamping force, or increase the clamping force. Enhance the surface quality of the parting lines, ejector pins and holes.
Short shot This is the phenomenon where molten plastics does not fill the mold cavity completely. and the portion of parts becomes incomplete shape. Cause The shot volume or injection pressure is not sufficient. Injection speed is so slow that the molten plastics becomes solid before it flows to the end of the mold. Solution Apply higher injection pressure. Install air vent or degassing device. Change the shape of the mold or gate position for better flow of the plastics.
Warpage This deformation appears when the part is removed from the mold and pressure is released. Cause Uneven shrinkage due to the mold temperature difference (surface temperature difference at cavity and core), and the thickness difference in the part. Injection pressure was too low and insufficient packing. Solution Take a longer cooling time and lower the ejection speed. Adjust the ejector pin position or enlarge the draft angle. Examine the part thickness or dimension. Balance cooling lines. Increase packing pressure.
Sink marks -Equal cooling from the surface -Secondary flow -Collapsed surface Sink Mark tsts t t s < t
CAE (computer aided engineering) Process simulation Material data base CAD MOLDFLOW C-Flow
Considerations in design of injection molded parts Guideline (3) gate location determines weld lines weld lines * Source: http://www.idsa-mp.org/proc/plastic/injection/injection_design_7.htmhttp://www.idsa-mp.org/proc/plastic/injection/injection_design_7.htm
Injection Molding: molds with moving cores and side-action cams - If the geometry of the part has undercuts [definition ?]
Mold Structure: Undercut, Slide core
Designing injection molds: typical features [source: www.idsa-mp.org]